Effect of High-Energy Ball Milling on the Magnetic ...· High-energy ball milling is a simple,...
Embed Size (px)
Transcript of Effect of High-Energy Ball Milling on the Magnetic ...· High-energy ball milling is a simple,...
Journal of Materials Science and Chemical Engineering, 2015, 3, 50-55 Published Online August 2015 in SciRes. http://www.scirp.org/journal/msce http://dx.doi.org/10.4236/msce.2015.38008
How to cite this paper: Gao, S., Song, S.H. and Song, Q.G. (2015) Effect of High-Energy Ball Milling on the Magnetic Proper-ties of NiZn Ferrite Ceramics Synthesized by Spark Plasma Sintering. Journal of Materials Science and Chemical Engineering, 3, 50-55. http://dx.doi.org/10.4236/msce.2015.38008
Effect of High-Energy Ball Milling on the Magnetic Properties of NiZn Ferrite Ceramics Synthesized by Spark Plasma Sintering Shang Gao, Shenhua Song*, Qingguo Song Shenzhen Key Laboratory of Advanced Materials, Shenzhen Graduate School, Harbin Institute of Technology, Shenzhen, China Email: *email@example.com, firstname.lastname@example.org Received 13 July 2015; accepted 9 August 2015; published 12 August 2015
Copyright 2015 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY). http://creativecommons.org/licenses/by/4.0/
Abstract High-density fine-grained Ni0.5Zn0.5Fe2O4 ferrite ceramics were synthesized by spark plasma sin-tering (SPS) in conjunction with high energy ball milling. The precursor powders were milled for 20 h, 40 h, and 60 h, respectively, and the milled powders were all sintered for 5 min at 900C. All the samples exhibit a single spinel phase. With increasing of the ball milling time, the relative den-sity of the samples increases (up to 97.7%), however, the grain size decreases (down to ~200 nm). At room temperature, the sample from the 40 h-milled powder has the best combination of satu-ration magnetization and coercivity (83 emu/g and 15 Oe). These outstanding magnetic proper-ties may be associated with high density and uniform microstructure created by SPS on the basis of fine precursor powders produced by high-energy ball milling.
Keywords Ferrites, Functional Materials, Magnetic Materials
1. Introduction Spinel ferrites constitute an important class of magnetic materials. Their applications always demand for high- density, low-porosity and controlled-microstructure. NiZn ferrite is one of them, which is commercially used in rod antennas, radio frequency circuits, transformer cores and read/write heads for high speed digital tape .
S. Gao et al.
The extensive application of NiZn ferrite is due to its remarkable magnetic behavior. Normally, conventional methods for preparation of ferrites involve high-temperatures and long-reaction times,
which would result in coarse-grained microstructures and poor magnetic properties. Conventional sintering for NiZn ferrite preparation usually requires temperatures up to 1300C for several hours even though small-sized powers are used . Recently, spark-plasma-sintering (SPS) is recognized as a novel sintering method of pre-paring ceramic materials because of even lower sintering temperature and shorter sintering time compared with microwave sintering and hot isostatic pressing -. Before SPS, the particle size of the powder is usually re-duced by high-energy ball milling which can also increase the homogeneity and reactivity of the mixture . High-energy ball milling is a simple, effective and productive way to produce various nano-crystal powders in high-energy planetary ball mills . High reactivity and small particle size can facilitate the production of high- density ceramics at low sintering temperatures . Therefore, the SPS along with high-energy ball milling has specific features of low sintering temperatures and short processing times. Until the present time, there have been limited reports on NiZn ferrite preparation by SPS . The aim of the present work is to fabricate a high- density fine-grained Ni0.5Zn0.5Fe2O4 ferrite material by SPS in conjunction with high-energy ball milling, em-phasizing the effect of ball milling on the magnetic properties of resulting ceramics.
2. Experimental Procedure The raw materials were reagent-grade NiO (>99.9%), ZnO (>99.9%), and Fe2O3 (>99.9%). Weighed powders according to the composition of Ni0.5Zn0.5Fe2O4 (abbreviated as NZF) were simply mixed in an evaporating dish and then milled thoroughly using a high-energy planetary ball mill with tungsten carbide (WC) bowls and balls in alcohol at a speed of 400 rpm for 20 h, 40 h and 60 h, respectively. The powders were dried at 80C for 2 h and observed by scanning electron microscopy (Hitachi S-4700 SEM). These powders were used as the precur-sor ones for SPS. They were placed in a graphite die and sintered at 900C for 5 min under a vacuum of 102 Pa by SPS. During the SPS, a pressure of 48 MPa was maintained. After the SPS, the prepared pellets with the size of 10 mm in diameter and 3 mm in thickness were annealed for 2 h at 50C lower than the SPS temperature to remove possible carbon contamination.
The phase purity and structure of the samples were analyzed by X-ray diffraction (XRD) using a Rigaku diffractometer (D/max 2500) with Cu-K radiation. Microstructures of the fracture surfaces were examined by SEM. Magnetic measurements were performed by a vibrating sample magnetometer (Lake Shore 7410 VSM).
3. Results and Discussion The morphologies of the powders milled for different times are shown in Figure 1. As seen, the powder par-ticles become finer and finer with increasing milling duration and their average size could be ~100 nm after 40 h milling. However, the 60 h-milled powder presents apparent agglomeration. It is anticipated that the 40 h-milled fine-sized powders are highly reactive and thereby can facilitate densification and homogenization of the sin-tered ceramics at a lower temperature.
The densities of the samples are represented in Figure 2(a). Clearly, the sample from the 20 h-milled powder has a density of 4.70 g/cm3, which is 89.4% of the theoretical density (5.26 g/cm3 ). With increasing mil-ling time, the density increases and reaches 5.10 g/cm3 when the milling time is 40 h. This value is equivalent to 97.0% of the theoretical density. The density can further increase slightly to 5.14 g/cm3 with longer milling time to 60 h although there is agglomeration of the powder particles. Consequently, the high-energy ball
Figure 1. Morphologies of the powder particles after high energy ball milling for (a) 20 h; (b) 40 h; and (c) 60 h.
S. Gao et al.
Figure 2. (a) The densities of the Ni0.5Zn0.5Fe2O4 ceramic samples prepared by SPS after high-energy ball milling for 20 h, 40 h, and 60 h (Dth = theoretical value); (b) The corresponding XRD patterns.
milling is an effective method of preparing the precursor powders in order to produce high-density ceramics. The XRD patterns of the samples presented in Figure 2(b) show that all the samples possess a spinel structure and there are no any secondary phases introduced during sintering.
Typical SEM images of the fracture surfaces of the samples are represented in Figure 3. Obviously, the mi-crostructure is quite uniform and increasingly dense with rising milling time. The grain size decreases gradually and linear intercept measurements indicate that the average values are approximately 300 nm, 250 nm and 200 nm for the milling times of 20 h, 40 h and 60 h, although there is some agglomeration in the 60 h-milled powder. This demonstrates that the sufficient high-energy ball milling may considerably promote densification and ho-mogenization in the SPS process with a reduction in average grain size. Usually, the ultrafine-grained structure of the SPS-prepared ceramics cannot be achieved by conventional sintering. The conventional sintering usually leads to a grain size of ~2 m , and even the microwave sintering usually results in a grain size of 1 - 2 m .
Magnetic hysteresis loops of the samples are shown in Figure 4(a). Clearly, these loops have typical charac-teristics of soft magnetic materials. The coercivity (Hc) is small and the saturation magnetization (Ms) is high. The narrow hysteresis loop indicates that the amount of dissipated energy in repeatedly reversing the magnetiza-tion is small, which is desirable for soft magnetic applications.
The values of Ms and Hc extracted from Figure 4(a) are shown in Figure 4(b) and Figure 4(c). As seen, the Ms increases with increasing milling time and may reach 83 and 86 emu/g for the samples prepared from the powders milled for 40 and 60 h, respectively. Nevertheless, the Hc of the sample from the 40 h-milled powder has a minimum value of 15 Oe, which is much lower than those from the other powders (19 Oe and 23 Oe). It is widely recognized  that the high density of soft magnetic material is beneficial to its magnetic properties for a high magnetization and low coercivity. Also, as far as the grain size effect is concerned, the coupling effect of ferromagnetic exchange between the grains may considerably reduce the magnetocrystalline anisotropy of local regions within the grains when the grain size approaches the single-domain size (~50 nm ), leading to en-hancement of the soft magnetic properties of the material . Consequently, the smaller the grain size, the bet-ter the magnetic properties become. When the grain size is beyond the single-domain